95 METALURGIJA 54 (2015) 1, 95-97
B. OLEKSIAK, M. KOZIOŁ, J. WIECZOREK, M. KRUPA, P. FOLĘGA
STRENGTH OF BRIQUETTES MADE OF CU CONCENTRATE
AND CARBON-BEARING MATERIALS
Received – Prispjelo: 2014-01-30 Accepted – Prihvaćeno: 2014-08-20 Preliminary Note – Prethodno priopćenje ISSN 0543-5846 METABK 54(1) 95-97 (2015) UDC – UDK 669.3:66.082:622.66:662.8.05=111
B. Oleksiak, M. Kozioł, J. Wieczorek, M. Krupa, P. Folęga - Silesian University of Technology, Katowice, Poland
In the present paper, results of the research on application of residual fine-grained, carbon-bearing materials as coke substitutes in the shaft process of copper matter smelting are discussed. The addition was introduced into the charge as a component of concentrate-made briquettes; then, its effects on properties of the obtained briquettes were analysed for their compressive and drop strengths. The results of investigations confirmed the potential use of proposed alternative fuels (as briquette components) in the process of copper matte smelting.
Keywords: copper concentrate, alternative fuel, briquette strength
In many pyrometallurgical processes, a major com-ponent of the charge, in addition to metal-bearing mate-rials, is coke or coke breeze. They are mainly energy carriers and reducers. For many years, extensive re-search on the use of cheaper substitutes for these mate-rials in metallurgical systems has been conducted. It involves iron ore sintering, the blast-furnace process and non-ferrous metal smelting in shaft furnaces as well as the technology of processing of various secondary metallurgical materials [1-5]. As alternative fuels for metallurgical processes, fine-grained, metal-bearing materials from the process of coal-enrichment, coke waste and biomass are applied. Some of them have al-ready been used for energy industry purposes. [6-8]. It should be noted, however, that alternative fuels must ensure a proper course of the specific technological pro-cess and should not compromise its thermal balance or cause extra consumption of fluxes and generation of larger slag amounts. In many metallurgical systems, physical properties of the fuel (coke, coke breeze) are of very high importance as they markedly affect e.g. gas permeability of the charge. It can be assumed that the above carbon-bearing materials and biomass are pro-spective fuels but in most cases, their application re-quires using charge materials in the form of granules, briquettes, pellets etc.
For the investigations, sulphide copper concentrate from “KGHM Mied ”, containing 27,81 % mass Cu, was used. The residual carbon-bearing materials were:
coal flotation concentrate, coke dust and anthracite dust. Their chemical compositions are presented in Ta-ble 1.
The briquetting process was conducted using a hy-draulic press (max force 10Mg).
Table 1 Chemical compositions of the investigated carbon-bearing materials
Fuel type Fractions of individual components / % mass
C S humidity ash
Coal l otation concentrate
64,3 0,45 26,5 8,71
Coke dust 88,5 0,6 0,3 10,3
Anthracite dust 71,5 1,7 5,4 25,1
The binder was sulphite liquor. The resulting bri-quettes were of a cylindrical shape, 30 mm in diameter and 25 - 30 mm in height (Figure 1). The sulphite liquor content in the briquetting mix corresponded to the in-dustrial values. In Table 2, compositions of the mixes used for the briquetting process are presented. The frac-tion of binder was 5,3 % mass in each case.
96 METALURGIJA 54 (2015) 1, 95-97 B. OLEKSIAK et al.: STRENGTH OF BRIQUETTES MADE OF CU CONCENTRATE AND CARBON-BEARING MATERIALS
The briquettes were tested for compressive strength and drop strength. The compressive strength test in-volved applying a load that caused fine grains to ap-proach each other. The compressive strength is capacity of a material to withstand loads tending to destroy it. It can be measured by plotting the applied compression force that led to destruction of the material structure against the surface affected by the compression force [9-11]. It should be noted that the test results depend on many factors, such as the shape, size and weight of the briquette as well as on the speed of the compressive head. Sufficiently high forces lead to briquette crack providing it is brittle enough. Certain briquette types with bitumen, clay or plastic material additives show plastic properties that preclude precise determination of the destructive force during compression. It should be noted that comparison of compression forces is possible for samples of the same shapes and sizes . The com-pressive strength depends on the direction of force act-ing on the material fibres or layers. In the case of fine-grained materials, it also depends on the material hu-midity and the temperature. For briquettes made of waste materials, the axial compressive strength values range widely from 0,5 MPa to 15 MPa and more . The copper concentrate briquettes were tested for com-pressive strength using the INSTRON 4469 test ma-chine at a compression speed of 2 mm/min.
In the drop strength test, 3 briquettes were dropped seven times onto a steel plate from a 2-metre height. After each drop, the amount of remaining briquette fraction (over 10 mm in diameter) was determined. The tested samples were both immediate and seasoned bri-quettes due to the fact that in the technological process, the manufactured briquettes must be sometimes stored for several days. This means that briquettes must show specific mechanical properties for a longer period.
STUDY RESULTS AND DISCUSSION
In Figure 2, examples of changes of compressive strengths in the case of immediate and seasoned (1-5 days) briquettes are presented. For all briquette batches, the strength was higher than 1 MPa and com-parable to the values for briquettes made of copper con-centrate only (as in the industrial setting). The data
show that for all investigated mixes, no strength deteri-oration with the seasoning period elongation was ob-served, which means that the briquettes can be success-fully stored before smelting, if required.
Table 3 shows examples of drop strength test results for the obtained briquettes. The strength is presented as a fraction of briquettes of over 10 mm in diameter in
Table 2 Compositions of the mixes used for the briquetting process
Concentrate fraction / %mass
Carbon-bearing material fraction / % mass
coal l otation concentrate
S 94,7 - -
-A-4 90,7 - - 4,0
C-4 90,7 - 4,0
-F-4 90,7 4,0 -
-A-2 90,7 - - 2,0
C-2 90,7 - 2,0
-F-2 90,7 2,0
-Figure 2 Compressive strength changes observed
in the obtained briquettes.
Compressive strength / MPa
Seasoning period / day
Table 3 Drop strength test results for the obtained briquettes
Type of the mix
Seasoning period / day
0 1 2 3 4 7
Content of the fraction over 10 mm / %
S 80,9 80,8 96,3 85,1 81,4 91,3
A-4 73,5 77,1 86,3 93,6 94,3 94,8
C-4 80,5 97,2 97,3 99,4 96,7 99,0
F-4 98,9 99,7 99,5 99,8 99,7 99,8
A-2 72,3 62,1 71,9 78,3 88,2 80,6
C-2 65,7 67,2 63,9 67,3 78,0 70,1
F-2 72,3 73,4 75,4 88,7 82,3 83,4
Content of the fraction over
Seasoning period / day
Figure 3 Drop strengths of selected briquettes versus the
97 METALURGIJA 54 (2015) 1, 95-97
B. OLEKSIAK et al.: STRENGTH OF BRIQUETTES MADE OF CU CONCENTRATE AND CARBON-BEARING MATERIALS
relation to the total briquette bulk. A graphic interpreta-tion of the results is presented in Figure 3. The Table 3 data refer to the strength after three drops as this value was assumed to illustrate briquette transport in the pe-riod from the immediate manufacturing completion to the shaft furnace charging (in the industrial setting).
Based on the investigations, it was concluded that: – It is possible to use fine-grained, carbon-bearing
materials as components of briquettes, obtained from copper concentrates, in the process of copper matte smelting in the shaft furnace.
– Introduction of a mix of alternative fuels into the briquetting process, in the amounts up to 4 %, ena-bles production of briquettes that show technolog-ically demanded compressive and drop strength properties.
– Humidity of the mix used for briquetting should not be higher than 10 %.
The study was conducted under the Research Project No. PST1/A5/21/2012, financed by the National Re-search and Development Centrethe – Poland.
 R. Findorák, M. Fröhlichová, J. Legemza, The effect of charcoal addition on iron-ore sintering emision, Conferen-ce proConferen-ceedings 13th Internat. Scientific GeoconferenConferen-ce Science and Technologies in Geology, Exploration and Mining, Albena (Bulgaria), 2(2013), 629-635.
 J. Legemza, M. Fröhlichová, R. Findorák, Thermodynamic study of utilization of charcoal in the iron-ore sintering pro-cess, Conference proceedings 13th International Scientific
Geoconference Science and Technologies in Geology, Ex-ploration and Mining, Albena (Bulgaria), 2 (2013), 649-656.  M. Niesler, J. Stecko, L. Blacha, B. Oleksiek, Application
of fine-grained coke breeze fractions in the process of iron sintering, Metalurgija, 53 (2014) 1, 37-40.
 J. Lipart, T. Matuła, M. Niesler, L. Blacha, J. Filipczyk, Wastes from the coal-enrichment process as alternative re-ducers for lead smelting from lead-acid accmulator scrap, Metalurgija, 52 (2013) 4, 493-496.
 J. Łabaj, M. Słowikowski, W. ymła, J. Lipart, The rese-arch on reactivity of alternative carbon reducers, Metalur-gija, 52 (2013) 1, 68-70.
 J. Hehlmann, W. Szeja, M. Jodkowski, P. Benducki, Rese-arch on Receiving Composite Energetic Biofuel Based on Biomass from Sewage Sludge Fermentation Process, Rocznik Ochrona rodowiska, 13 (2011) 1, 921-934.  J. Tomeczek, S. Gil, The kinetics of coal chars
hydrogasi-fication, Fuel Processing Technology, Elsevier, 91 (2010) 11, 1564-1568.
 S. Gil, P. Mocek, W. Bialik, Changes in total active centres on particle surfaces during coal pyrolysis, gasification and combustion, Chemical and Process Engineering, 32 (2011) 2, 155-169.
 J. Myalski, J. Wieczorek, A. Płachta, Physical and Mecha-nical Properties of Composites with Aluminum Alloy Ma-trix Designed for Metal Forming, Solid State Phenomena, 212 (2013), 59-62.
 M. Koziol, Experimental study on the effect of stitch ar-rangement on mechanical performance of GFRP laminates manufactured on a basis of stitched preforms, Journal of Composite Materials, 46 (2012) 9, 1067-1078.
 M. Koziol, Effect of thread tension on mechanical perfor-mance of stitched glass fibre-reinforced polymer laminates – experimental study, Journal of Composite Materials, 47 (2013) 16, 1919-1930.
 G. Borowski, Wykorzystanie brykietowania do zagospo-darowania odpadów, Monografia. Lubelskie Towarzystwo Naukowe, Lublin, 2011.
 G. Borowski, M. Miłczak, Badania przydatno ci brykietów
z popiołów paleniskowych jako podbudowy drogowe,
Postępy Nauki i Techniki, 4 (2010), 136-143.